# MEC 302 Mechanics of Materials - 02-Part 1

```ADU
Lecture
MEC 302
1
2
Mechanics Of Materials
MEC 302
MEC 302
2
Tentative Lectures Schedule
Topic
Introduction Concept of Stress,
1.1-1.7
Introduction Concept of Stress
Torsion,
Torsion
Pure Bending,
Analysis and Design of Beams for Bending,
Shearing Stresses in Beams and Thin-Walled Members
Transformations of Stress and Strain,
Transformations of Stress and Strain,
Deflections of Beams
Deflections of Beams
Columns (Buckling) ,
Final Exam
1.8-1.13
2.1-2.10
2.11-2.19
3.1-3.5
3.6-3.8
4.1-4.7,
5.1-5.4
6.1-6.7,
7.1-7.3
7.4-7.9
9.1-9.5
9.7
10.1-10.6
2
Lecture 2
MEC 302
3
Lecture 2
MEC 302
4
Lecture 2

MEC 302
5
5
Lecture 2

MEC 302
6
6
Lecture 2
MEC 302
7
7
Lecture 2
MEC 302
8
2.3 STRESS-STRAIN DIAGRAM
 We saw in Sec. 2.2 that the diagram representing the
relation between stress and strain in a given material
is an important characteristic of the material.
 To obtain the stress-strain diagram of a material, one
usually conducts a tensile test on a specimen of the
material.
 One type of specimen commonly used is shown in
Photo 2.1.
 The cross-sectional area of the cylindrical central
portion of the specimen has been accurately
determined and two gage marks have been inscribed
on that portion at a distance L0 from each other.
 The distance L0 is known as the gage length of the
specimen.
 The test specimen is then placed in a testing machine
(Photo 2.2),which is used to apply a centric load P.
As the load P increases, the distance L between the
two gage marks also increases (Photo 2.3).
8
Lecture 2
MEC 302
9
2.3 STRESS-STRAIN DIAGRAM
9
Lecture 2

MEC 302
10
2.3 STRESS-STRAIN DIAGRAM
10
Lecture 2
11
MEC 302
2.3 STRESS-STRAIN DIAGRAM
 It is possible, however, to distinguish some common
characteristics among the stress-strain diagrams of
various groups of materials and to divide materials
into two broad categories on the basis of these
characteristics, namely, the ductile materials and the
brittle materials.
 Ductile materials, which comprise structural steel, as
well as many alloys of other metals, are characterized
by their ability to yield at normal temperatures.
 As the specimen is subjected to an increasing load, its
length first increases linearly with the load and at a
very slow rate.
 Thus, the initial portion of the stress-strain diagram is
a straight line with a steep slope (Fig. 2.6).
 However, after a critical value σY of the stress has
been reached, the specimen undergoes a large
deformation with a relatively small increase in the
 This deformation is caused by slippage of the material
along oblique surfaces and is due, therefore, primarily
to shearing stresses.
11
Lecture 2
MEC 302
12
Lecture 2
13
MEC 302
2.3 STRESS-STRAIN DIAGRAM
 As we can note from the stress-strain diagrams of
two typical ductile materials (Fig. 2.6), the
elongation of the specimen after it has started to
yield can be 200 times as large as its deformation
before yield.
 After a certain maximum value of the load has
been reached, the diameter of a portion of the
specimen begins to decrease, because of local
instability (Photo 2.4a). This phenomenon is
known as necking.
 After necking has begun, somewhat lower loads
are sufficient to keep the specimen elongating
further, until it finally ruptures (Photo 2.4b).
 We note that rupture occurs along a cone-shaped
surface that forms an angle of approximately 45o
with the original surface of the specimen.
 This indicates that shear is primarily responsible
for the failure of ductile materials.
13
Lecture 2
14
MEC 302
2.3 STRESS-STRAIN DIAGRAM
 This confirms the fact that, under an axial load,
shearing stresses are largest on surfaces forming an
angle of 45o with the load (cf. Sec. 1.11).
 The stress σY at which yield is initiated is called the
yield strength of the material, the stress σU
corresponding to the maximum load applied to the
specimen is known as the ultimate strength, and the
stress σB corresponding to rupture is called the
breaking strength.
 Brittle materials, which comprise cast iron, glass, and
stone, are characterized by the fact that rupture occurs
without any noticeable prior change in the rate of
elongation (Fig. 2.7).
 Thus, for brittle materials, there is no difference
between the ultimate strength and the breaking
strength. Also, the strain at the time of rupture is much
smaller for brittle than for ductile materials.
14
Lecture 2
MEC 302
15
Lecture 2
16
MEC 302
2.3 STRESS-STRAIN DIAGRAM
 From Photo 2.5, we note the absence of any necking of
the specimen in the case of a brittle material, and
observe that rupture occurs along a surface
 We conclude from this observation that normal
stresses are primarily responsible for the failure of
brittle materials.
 The stress-strain diagrams of Fig. 2.6 show that
structural steel and aluminum, while both ductile,
have different yield characteristics.
 In the case of structural steel (Fig. 2.6a), the stress
remains constant over a large range of values of the
strain after the onset of yield.
 Later the stress must be increased to keep elongating
the specimen, until the maximum value σU has been
reached.
 This is due to a property of the material known as
strain-hardening.
16
Lecture 2
17
MEC 302
2.3 STRESS-STRAIN DIAGRAM
 The yield strength of structural steel can be
determined during the tensile test by watching the
load shown on the display of the testing machine.
suddenly drop to a slightly lower value, which is
maintained for a certain period while the specimen
keeps elongating.
 In a very carefully conducted test, one may be able to
distinguish between the upper yield point, which
corresponds to the load reached just before yield
starts, and the lower yield point, which corresponds
to the load required to maintain yield.
 Since the upper yield point is transient, the lower
yield point should be used to determine the yield
strength of the material.
17
Lecture 2

MEC 302
18
2.3 STRESS-STRAIN DIAGRAM
18
Lecture 2
MEC 302
19
Lecture 2
 A standard measure of the ductility of a
material is its percent elongation, which is
defined as
 Another measure of ductility which is
sometimes used is the percent reduction in
area, defined as
MEC 302
20
2.3 STRESS-STRAIN DIAGRAM
20
Lecture 2
21
MEC 302
2.3 STRESS-STRAIN DIAGRAM
 Thus far, we have discussed only tensile tests. If a
 The stress-strain curve obtained would be essentially
the same through its initial straight-line portion and
through the beginning of the portion corresponding
to yield and strain-hardening.
 Particularly noteworthy is the fact that for a given
steel, the yield strength is the same in both tension
and compression.
 For larger values of the strain, the tension and
compression stress-strain curves diverge, and it
should be noted that necking cannot occur in
compression.
21
Lecture 2
22
MEC 302
2.3 STRESS-STRAIN DIAGRAM
 For most brittle materials, one finds that the ultimate
strength in compression is much larger than the
ultimate strength in tension.
 This is due to the presence of flaws, such as
microscopic cracks or cavities, which tend to weaken
the material in tension, while not appreciably affecting
its resistance to compressive failure.
 An example of brittle material with different
properties in tension and compression is provided by
concrete, whose stress-strain diagram is shown in Fig.
2.9.
 On the tension side of the diagram, we first observe a
linear elastic range in which the strain is proportional
to the stress.
 After the yield point has been reached, the strain
increases faster than the stress until rupture occurs.
22
Lecture 2
 The behavior of the material in compression is
different. First, the linear elastic range is significantly
larger.
 Second, rupture does not occur as the stress reaches
its maximum value. Instead, the stress decreases in
magnitude while the strain keeps increasing until
rupture occurs.
 Note that the modulus of elasticity, which is
represented by the slope of the stress-strain curve in
its linear portion, is the same in tension and
compression. This is true of most brittle materials.
MEC 302
23
2.3 STRESS-STRAIN DIAGRAM
23
Lecture 2
MEC 302
24
Lecture 2
25
MEC 302
2.4 TRUE STRESS AND TRUE STRAIN
 We recall that the stress plotted in the diagrams of
Figs. 2.6 and 2.7 was obtained by dividing the load P
by the cross-sectional area A0 of the specimen
measured before any deformation had taken place.
 Since the cross-sectional area of the specimen
decreases as P increases, the stress plotted in our
diagrams does not represent the actual stress in the
specimen.
 The difference between the engineering stress σ =
P/A0 that we have computed and the true stress σt =
P/A obtained by dividing P by the cross-sectional
area A of the deformed specimen becomes apparent
in ductile materials after yield has started.
25
Lecture 2

MEC 302
26
2.4 TRUE STRESS AND TRUE STRAIN
26
Lecture 2

MEC 302
27
2.4 TRUE STRESS AND TRUE STRAIN
27
Lecture 2

MEC 302
28
2.5 HOOKE’S LAW; MODULUS OF ELASTICITY
28
Lecture 2

MEC 302
29
2.5 HOOKE’S LAW; MODULUS OF ELASTICITY
29
Lecture 2
MEC 302
30
Lecture 2
MEC 302
Anisotropic Materials Consists of Fiberreinforced
Composite Materials
31
Lecture 2
32
MEC 302
2.6 ELASTIC VERSUS PLASTIC BEHAVIOR OF A MATERIAL
 If the strains caused in a test specimen by the
application of a given load disappear when the
load is removed, the material is said to behave
elastically.
 The largest value of the stress for which the
material behaves elastically is called the elastic
limit of the material.
 If the material has a well-defined yield point as
in Fig. 2.6a, the elastic limit, the proportional
limit (Sec. 2.5), and the yield point are
essentially equal.
 In other words, the material behaves elastically
and linearly as long as the stress is kept below
the yield point.
32
Lecture 2

MEC 302
33
2.6 ELASTIC VERSUS PLASTIC BEHAVIOR OF A MATERIAL
33
Lecture 2
MEC 302
2.6 ELASTIC VERSUS PLASTIC BEHAVIOR OF A MATERIAL
34
Lecture 2
35
MEC 302
2.6 ELASTIC VERSUS PLASTIC BEHAVIOR OF A MATERIAL
 When a material does not possess a well-defined
yield point, the elastic limit cannot be determined
with precision.
 However, assuming the elastic limit equal to the yield
strength as defined by the offset method (Sec. 2.3)
results in only a small error.
 Indeed, referring to Fig. 2.8, we note that the
straight line used to determine point Y also
stress σY has been reached.
 While the material does not behave truly elastically,
the resulting plastic strain is as small as the selected
offset.
almost reaches point C.
35
Lecture 2
36
MEC 302
2.6 ELASTIC VERSUS PLASTIC BEHAVIOR OF A MATERIAL
 It will then bend to the right and connect with the
curved portion of the original stress-strain diagram.
 We note that the straight-line portion of the new
of the initial one.
 Thus, the proportional limit and the elastic limit have
increased as a result of the strain-hardening that
 However, since the point of rupture R remains
unchanged, the ductility of the specimen, which should
now be measured from point D, has decreased.
 We assume that the material is mild steel, for which
the yield strength is the same in tension and in
compression.
36
Lecture 2
MEC 302
2.6 ELASTIC VERSUS PLASTIC BEHAVIOR OF A MATERIAL
37
Lecture 2
38
MEC 302
2.6 ELASTIC VERSUS PLASTIC BEHAVIOR OF A MATERIAL
 The initial load is tensile and is applied until point C
has been reached on the stress-strain diagram (Fig.
2.15).
applied, causing the material to reach point H, where
the stress change is equal to 2σY.
 We note that portion DH of the stress-strain diagram is
curved and does not show any clearly defined yield
point.
 This is referred to as the Bauschinger effect. As the
compressive load is maintained, the material yields
along line HJ.
 If the load is removed after point J has been reached,
the stress returns to zero along line JK, and we note
that the slope of JK is equal to the modulus of
elasticity E.
38
Lecture 2
39
MEC 302
2.6 ELASTIC VERSUS PLASTIC BEHAVIOR OF A MATERIAL
 The resulting permanent set AK may be positive,
negative, or zero, depending upon the lengths of the
segments BC and HJ.
 If a tensile load is applied again to the test specimen,
the portion of the stress-strain diagram beginning at K
(dashed line) will curve up and to the right until the
yield stress σY has been reached.
place along line C’D’.
 As the reverse load is applied, the stress becomes
compressive, reaching its maximum value at H’ and
maintaining it as the material yields along line H’J’.
 We note that while the maximum value of the
compressive stress is less than σY, the total change in
stress between C’ and H’ is still equal to 2σY
39
Lecture 2
40
MEC 302
2.6 ELASTIC VERSUS PLASTIC BEHAVIOR OF A MATERIAL
 If point K or K’ coincides with the origin A of the
diagram, the permanent set is equal to zero, and the
specimen may appear to have returned to its original
condition.
 However, internal changes will have taken place and,
specimen will rupture without any warning after
relatively few repetitions.
 This indicates that the excessive plastic deformations
to which the specimen was subjected have caused a
radical change in the characteristics of the material.
seldom allowed, and only under carefully controlled
conditions.
 Such situations occur in the straightening of damaged
material and in the final alignment of a structure or
machine.
40
Lecture 2
MEC 302
2.6 ELASTIC VERSUS PLASTIC BEHAVIOR OF A MATERIAL
41
Lecture 2
42
MEC 302
 As we know that if the maximum stress in the specimen
does not exceed the elastic limit of the material, the
specimen returns to its initial condition when the load is
removed.
repeated many times, provided that the stresses remain
in the elastic range.
dozen or even a few hundred times.
 However, as you will see, it is not correct when loadings
are repeated thousands or millions of times.
 In such cases, rupture will occur at a stress much lower
than the static breaking strength σB; this phenomenon
is known as fatigue.
 Hence a fatigue failure is of a brittle nature, even for
materials that are normally ductile.
42
Lecture 2
43
MEC 302
 Fatigue must be considered in the design of all
structural and machine components that are
subjected to repeated or to fluctuating loads.
expected during the useful life of a component
varies greatly.
 For example, a beam supporting an industrial
crane may be loaded as many as two million times
half a billion times if the automobile is driven
200,000 miles, and an individual turbine blade
may be loaded several hundred billion times
43
Lecture 2
44
MEC 302
failure of a specimen through repeated successive
experimentally for any given maximum stress level.
 If a series of tests is conducted, using different
maximum stress levels, the resulting data may be
plotted as a σ-n (S-N) curve.
 For each test, the maximum stress σ is plotted as an
ordinate and the number of cycles n as an abscissa;
because of the large number of cycles required for
rupture, the cycles n are plotted on a logarithmic
scale.
 A typical σ-n curve for steel is shown in Fig. 2.16.
We note that, if the applied maximum stress is high,
relatively few cycles are required to cause rupture.
44
Lecture 2
45
MEC 302
 As the magnitude of the maximum stress is reduced,
the number of cycles required to cause rupture
increases, until a stress, known as the endurance limit,
is reached.
 The endurance limit is the stress for which failure does
not occur, even for an indefinitely large number of
 For a low-carbon steel, such as structural steel, the
endurance limit is about one-half of the ultimate
strength of the steel.
 For nonferrous metals, such as aluminum and copper,
a typical σ-n curve (Fig. 2.16) shows that the stress at
cycles is increased.
 For such metals, one defines the fatigue limit as the
stress corresponding to failure after a specified
45
Lecture 2
MEC 302
46
Lecture 2
MEC 302
47
Lecture 2

MEC 302
48
Variable Cross-sectional Area
48
Lecture 2
Example 2.01
SOLUTION:
Divide the rod into components at the
Apply a free-body analysis on each
component to determine the
internal force
MEC 302
E  200GPa
Evaluate the total of the component
deflections.
Determine the
deformation of the steel
rod shown under the
3- 49
Lecture 2
Example 2.01
SOLUTION:
Divide the rod into three
components:
Apply free-body analysis to each component
to determine internal forces,
P1  240 kN
P2  60 kN
P3  120 kN
MEC 302
Evaluate total deflection,
L1  L2  300 mm.
L3  400 mm.
A1  A2  580 mm 2
A3  190 mm 2
  1.729 mm
3- 50
Lecture 2
51
MEC 302
Deformation is Measured by the Relative Displacement
 The deformation of the rod is measured by the
relative displacement of one end of the rod with
respect to the other
 Let us consider, for instance, the assembly shown in
Fig. 2.20a, which consists of three elastic bars of
length L connected by a rigid pin at A.
 If a load P is applied at B (Fig. 2.20b), each of the
three bars will deform.
 Since the bars AC and AC’ are attached to fixed
supports at C and C’, their common deformation is
measured by the displacement δA of point A.
 On the other hand, since both ends of bar AB move,
the deformation of AB is measured by the difference
between the displacements δA and δB of points A and
B, i.e., by the relative displacement of B with respect
to A.
51
Lecture 2
Denoting this relative displacement by δB/A, we write
MEC 302
52
Deformation is Measured by the Relative Displacement
52
Lecture 2
MEC 302
53
Lecture 2
MEC 302
54
Lecture 2
MEC 302
55
Lecture 2
The rigid castings A and B are connected by two 18 mm
diameter steel bolts CD and GH and are in contact with the
ends of a 38 mm diameter aluminum rod EF. Each bolt is
single-threaded with a pitch of 2.5 mm, and after being snugly
fitted, the nuts at D and H are both tightened one-quarter of a
turn. Knowing that E is 200 GPa for steel and 70 GPa for
aluminum, determine the normal stress in the rod.
56
Sample Problem 2.2
MEC 302
450 mm
300 mm
56
Lecture 2